# ch13

August 28, 2017 | Author: Juan Camilo Méndez | Category: Fibers, Extrusion, Thermoplastic, Plastic, Amorphous Solid

#### Description

13 SHAPING PROCESSES FOR PLASTICS Review Questions 13.1

What are some of the reasons why the plastic shaping processes are important? Answer. The reasons include (1) many of the processes are net shape processes; (2) in general, less energy is employed than in metalworking processes; (3) lower temperatures are required to process plastics than metals or ceramics; (4) there is great flexibility in geometry; and (5) painting and other finishing processes are generally not required.

13.2

Identify the main categories of plastics shaping processes, as classified by the resulting product geometry. Answer. The categories are (1) extrusion, (2) molding, (3) forming of continuous sheets and films, (4) fibers, (5) foamed products, and (6) discrete formed sheets and films.

13.3

Viscosity is an important property of a polymer melt in plastics shaping processes. Upon what parameters does viscosity depend? Answer. Viscosity of a polymer melt depends on (1) temperature and (2) shear rate. Also, (3) the molecular weight of the polymer affects viscosity.

13.4

How does the viscosity of a polymer melt differ from most fluids that are Newtonian. Answer. A polymer melt exhibits pseudoplasticity, which means that its value decreases with increasing shear rate.

13.5

What does viscoelasticity mean, when applied to a polymer melt? Answer. Viscoelasticity is a combination of viscous and elastic properties which cause the melt to exhibit memory - the tendency to return to its previous shape, as exhibited by die swell in extrusion.

13.6

Define die swell in extrusion. Answer. Die swell is the tendency of the extrudate to expand in cross-sectional dimensions immediately on exiting the die orifice. It results from the viscoelastic properties of the polymer melt.

13.7

Briefly describe the plastic extrusion process. Answer. In plastic extrusion, a polymer melt is compressed to flow through a die orifice and thus the continuous length of the plastic assumes a cross-sectional shape that is approximately the same as that of the orifice.

13.8

The barrel and screw of an extruder are generally divided into three sections; identify the sections. Answer. The sections are (1) the feed section, in which the feed stock is fed from the hopper and heated; (2) the compression section, in which the polymer changes to a viscous fluid; and (3) the metering section, in which pressure is developed to pump the plastic through the die orifice.

13.9

What are the functions of the screen pack and breaker plate at the die end of the extruder barrel? Answer. The functions are to (1) filter dirt and lumps, (2) build pressure, (3) straighten the flow and remove memory.

13.10 What are the various forms of extruded shapes and corresponding dies? Answer. The shapes are (1) solid profiles, such as rounds and L-shapes; (2) hollow profiles, such as tubes; (3) wire and cable coating; (4) sheet and film; and (5) filaments (continuous fibers). Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

62

63

64

65

13.1

The forward movement of polymer melt in an extruder barrel is resisted by drag flow, which is caused by the resistance to flow through the die orifice: (a) true or (b) false? Answer. (b). Drag flow is the forward motion of the melt caused by the Archimedian screw principle in the barrel. The resistance to forward flow is called back pressure flow.

13.2

Which of the following are sections of a conventional extruder barrel for thermoplastics (three best answers): (a) compression section, (b) die section, (c) feed section, (d) heating section, (e) metering section, and (f) shaping section? Answer. (a), (c), and (e).

13.3

Which of the following processes are associated with the production of plastic sheet and film (three correct answers): (a) blown-film extrusion process, (b) calendering, (c) chill-roll extrusion, (d) doctor blade method, (e) spinning, (f) thermoforming, (g) transfer molding? Answer. (a), (b), and (c).

13.4

The principal components of an injection molding machine are which two of the following: (a) clamping unit, (b) hopper, (c) injection unit, (d) mold, and (e) part ejection unit? Answer. (a) and (c).

13.5

The parting line in injection molding is which one of the following: (a) the lines formed where polymer melt meets after flowing around a core in the mold, (b) the narrow gate sections where the parts are separated from the runner, (c) where the clamping unit is joined to the injection unit in the molding machine, or (d) where the two mold halves come together? Answer. (d).

13.6

The function of the ejection system is which one of the following: (a) move polymer melt into the mold cavity, (b) open the mold halves after the cavity is filled, (c) remove the molded parts from the runner system after molding, or (d) separate the part from the cavity after molding? Answer. (d).

13.7

A three-plate mold offers which of the following advantages when compared to a two-plate mold (two best answers): (a) automatic separation of parts from runners, (b) gating is usually at the base of the part to reduce weld lines, (c) sprue does not solidify, and (d) stronger molded parts? Answer. (a) and (b).

13.8

Which of the following defects or problems is associated with injection molding (three correct answers): (a) bambooing, (b) die swell, (c) drag flow, (d) flash, (e) melt fracture, (f) short shots, or (g) sink marks? Answer. (d), (f), and (g).

13.9

In rotational molding, centrifugal force is used to force the polymer melt against the surfaces of the mold cavity where solidification occurs: (a) true or (b) false? Answer. (b). It is the force of gravity in the doubly rotating mold that forces the polymer against the mold surfaces.

13.10 Use of a parison is associated with which one of the following plastic shaping processes: (a) bi-injection molding, (b) blow molding, (c) compression molding, (d) pressure thermoforming, or (e) sandwich molding? Answer. (b). 13.11 A thermoforming mold with a convex form is called which one of the following (may be more than one): (a) a die, (b) a negative mold, (c) a positive mold, or (d) a three-plate mold? Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

66

Answer. (c). 13.12 The term encapsulation refers to which one of the following plastics shaping processes: (a) casting, (b) compression molding, (c) extrusion of hollow forms, (d) injection molding in which a metal insert is encased in the molded part, or (e) vacuum thermoforming using a positive mold? Answer. (a). 13.13 The two most common polymer foams are which of the following: (a) polyacetal, (b) polyethylene, (c) polystyrene, (d) polyurethane, and (e) polyvinylchloride? Answer. (c) and (d). 13.14 In which of the following property categories do plastic parts often compare favorably with metals (two best answers): (a) impact resistance, (b) resistance to ultraviolet radiation, (c) stiffness, (d) strength, (e) strength-to- weight ratio, or (f) temperature resistance? Answer. (a) and (e). 13.15 Which of the following processes are generally limited to thermoplastic polymers (two best answers): (a) blow molding, (b) compression molding, (c) reaction injection molding, (d) thermoforming, (e) transfer molding, (f) wire coating? Answer. (a) and (d). 13.16 Which of the following processes would be applicable to produce hulls for small boats (three best answers): (a) blow molding, (b) compression molding, (c) injection molding, (d) rotational molding, or (e) vacuum thermoforming? Answer. (a), (d), and (e).

Problems Extrusion 13.1

The diameter of an extruder barrel is 65 mm and its length = 1.75 m. The screw rotates at 55 rev/min. The screw channel depth = 5.0 mm, and the flight angle = 18°. The head pressure at the die end of the barrel is 5.0 x 106 Pa. The viscosity of the polymer melt is given as 100 Pas. Find the volume flow rate of the plastic in the barrel. Solution: Qd = 0.5π2(65x10-3)2(55/60)(5x10-3)sin 18 cos 18 = 95,560x10-9(0.3090)(0.9510) = 28.081 x 10-6 m3/s p = 5 MPa = 5x106 n/m2 Qb = π(5x106)(65x10-3)(5x10-3)3(sin 18)2/12(100)(1.75) = 5.804(10-6) m3/s Qx = 28.081 - 5.804 = 22.277 x 10-6 m3/s.

13.2

An extruder has a diameter of 5.0 in and a length to diameter ratio of 26. The barrel heats the polypropylene melt to 450°F, which provides a melt viscosity of 0.0025 lb-s/in2. The pitch of the screw is 4.2 in and the channel depth is 0.15 in. In operation the screw rotates at 50 rev/min and a head pressure of 450 lb/in2 is generated. What is the volume flow rate of polypropylene from the die at the end of the barrel? Solution: A = tan-1(p/(πD)) = tan-1(4.2/(5π)) = 15° Qd = 0.5π2 D2 N dc sinA cosA = 0.5π2 (5.02)(50/60) 0.15 sin 15 cos 15 = 3.9 in3/sec Qb = pπDdc3sin2A/(12ηL) = 450π(5.0)(0.153)sin215/(12(0.0025)(5.0)(26)) = 0.41 in3/sec Qx = Qd – Qb = 3.9 – 0.41 = 3.5 in3/sec

Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

67

13.3

An extruder barrel has a diameter of 110 mm and a length of 3.0 m. The screw channel depth = 7.0 mm, and its pitch = 95 mm. The viscosity of the polymer melt is 105 Pas, and the head pressure in the barrel is 4.0 MPa. What rotational speed of the screw is required to achieve a volumetric flow rate of 90 cm3/s? Solution: A = tan-1(p/(πD)) = tan-1(95/110π) = 15.37° Qd = 0.5π2 D2 N dc sinAcosA = 0.5π2(0.110)2(N)(7.0x10-3)sin 15.37 cos 15.37 = 106.8 N x 10-6 m3/s Qb = π(4x106)(0.110)(7x10-3)3(sin 15.37)2/12(105)(3.0) = 8.81 x 10-6 m3/s Qx = Qd - Qb = 106.8 N x 10-6 – 8.81 x 10-6 = 90 x 10-6 m3/s 106.8 N = 90.0 + 8.81 = 98.81 N = 98.81/106.8 = 0.9252 rev/s = 55.51 rev/min.

13.4

An extruder has a barrel diameter of 2.5 in and a length of 6.0 ft. The screw has a channel depth of 0.25 in, a flight angle of 20°, and rotates at 55 rev/min. The material being extruded is polypropylene. At the present settings, the volumetric flow rate of the polymer melt is 1.50 in3/sec and the head pressure is 500 lb/in2. (a) Under these operating characteristics, what is the viscosity of the polypropylene? (b) Using Figure 13.2, approximate the temperature in °F of the polypropylene. Solution: (a) Qd = 0.5π2 D2 Ndc sinA cosA = 0.5π2(2.52)(55/60)(0.25)sin 20 cos 20 Qd = 2.27 in3/sec Qb = Qd – Qx = 2.27 – 1.50 = 0.78 in3/sec η = pπDdc3 in2 A/(12 QbL) = 500π(2.5)(0.253)sin2(20)/(12(0.78)(6)(12)) = 0.011 lb-s/in2 (b) X-axis is Log scale. Therefore LOG(0.011) = -1.96 This is very close to –2, which is at the 10-2 hash mark on the y-axis. This yields about 410°F.

13.5

An extruder has diameter = 80 mm and length = 2.0 m. Its screw has a channel depth = 5 mm, flight angle = 18 degrees, and it rotates at 1 rev/sec. The plastic melt has a shear viscosity = 150 Pas. Determine the extruder characteristic by computing Qmax and pmax and then finding the equation of the straight line between them. Solution: Qmax = Qd = 0.5π2(0.08)2(1)(5x10-3)sin 18 cos 18 = 0.158 x 10-3(0.3090)(0.9510) = 46.4 x 10-6 m3/s pmax = 6π(0.08)(1)(2)(150)(cot 18)/(5x10-3)2 = 452.4(3.077)/25x10-6 = 55 x 106 Pa = 55 MPa Qx = 46.4 x 10-6 - (46.4x10-6/55)p Qx = 46.4 x 10-6 - 0.8436 x 10-6 p, where p has units of MPa

13.6

Determine the helix angle A such that the screw pitch p is equal to the screw diameter D. This is called the "square" angle in plastics extrusion - the angle that provides a flight advance equal to one diameter for each rotation of the screw. Solution: Assume flight land = zero. From Eq. (15.4), tan A = pitch/πD If pitch = D, then A = tan-1(1/π) = 17.66°

13.7

An extruder barrel has a diameter of 2.5 in. The screw rotates at 60 rev/min; its channel depth = 0.20 in, and its flight angle = 17.5°. The head pressure at the die end of the barrel is 800 lb/in2 and the length of the barrel is 50 in. The viscosity of the polymer melt is 122 x 10-4 lb-sec/in2. Determine the volume flow rate of the plastic in the barrel. Solution: Qd = 0.5π2(2.5)2(1)(.2)sin 17.5 cos 17.5 = 0.5(12.337)(0.3007)(0.9537) = 1.769 in3/sec Qb = π(800)(2.5)(.2)3(sin 17.5)2/12(122x10-4)(50) = 0.621 in3/sec Qx = 1.769 - 0.621 = 1.148 in3/sec.

Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

68

13.8

An extruder barrel has a diameter of 4.0 in and an L/D ratio of 28. The screw channel depth = 0.25 in, and its pitch = 4.8 in. It rotates at 60 rev/min. The viscosity of the polymer melt is 100 x 10-4 lb-sec/in2. What head pressure is required to obtain a volume flow rate = 150 in3/min? Solution: A = tan-1(pitch/πD) = tan-1(4.8/4π) = 20.9° Qd = 0.5π2(4)2(1)(0.25)sin 20.9 cos 20.9 = 19.74(0.3567)(0.9342) = 6.578 in3/sec = 394.66 in3/min Qx = Qd - Qb = 394.66 - Qd = 150 Qb = 394.66 - 150 = 244.66 in3/min = 4.078 in3/sec L = 4(28) = 112 in. Qb = πp(4)(0.25)3(sin 20.9)2/(12(100x10-4)(112)) = 4.078 0.0018592 p = 4.078 p = 2193.4 lb/in2

13.9

An extrusion operation produces continuous tubing with outside diameter = 2.0 in and inside diameter = 1.7 in. The extruder barrel has a diameter = 4.0 in and length = 10 ft. The screw rotates at 50 rev/min; it has a channel depth = 0.25 in and flight angle = 16°. The head pressure has a value of 350 lb/in2 and the viscosity of the polymer melt is 80 x 10-4 lb-sec/in2. Under these conditions, what is the production rate in length of tube/min, assuming the extrudate is pulled at a rate that eliminates the effect of die swell (i.e., the tubing has the same OD and ID as the die profile). Solution: Qd = 0.5π2(4)2(50/60)(.25)sin 16 cos 16 = 16.45(0.2756)(0.9613) = 4.358 in3/sec Qb = π(350)(4)(.25)3(sin 16)2/(12(80x10-4)(120)) = 0.453 in3/sec Qx = 4.358 - 0.453 = 3.905 in3/sec. Ax = 0.25π(22 - 1.72) = 0.872 in2 vx = 3.905/0.872 = 4.478 in/sec = 22.39 ft/min.

13.10 An extruder has barrel diameter and length of 100 mm and 2.8 m, respectively. The screw rotational speed = 50 rev/min, channel depth = 7.5 mm, and flight angle = 17°. The plastic melt has a shear viscosity = 175 Pas. Determine: (a) the extruder characteristic, (b) the shape factor Ks for a circular die opening with diameter = 3.0 mm and length = 12.0 mm, and (c) the operating point (Q and p). Solution: Qmax = Qd = 0.5π2(.1)2(50/60)(7.5x10-3) sin 17 cos 17 = 308.4 x 10-6(0.2924)(0.9563) = 86.2 x 10-6 m3/s pmax = 6π(.1)(50/60)(2.8)(175)(cot 17)/(7.5x10-3)2 = 44.75 x 106 Pa =44.75 MPa Qx = 86.2 x 10-6 - 1.926 x 10-12 p, where p has units of Pa (b) Given: Dd = 3 mm, Ld = 12 mm. Ks = π(3 x 10-3)4/(128(175)(12 x 10-3)) = 0.9467 x 10-12 (c) 0.9467 x 10-12 p = 86.2 x 10-6 - 1.926 x 10-12 p 2.8727 x 10-12 p = 86.2 x 10-6 p = 30.0 x 106 Pa = 30 MPa Qx = 0.9467 x 10-12 (30 x 106) = 28.4 x 10-6 m3/s Check with extruder characteristic: Qx = 86.2 x 10-6 - 1.926 x 10-12 (30 x 106) = 28.4 x 10-6 m3/s. 13.11 For Problem 13.10, assume the material is acrylic. (a) Using Figure 13.2, determine the temperature of the polymer melt. (b) If the temperature is lowered 20°C, estimate the resulting viscosity of the polymer melt. (hint: the y-axis of Figure 13.2 is a log scale, not linear). Solution: (a) When viscosity = 175 Pas, Log(175) = 2.243, and temperature is approximately 260°C. (b) At 240°C, Log(viscosity) is approximately 2.7 and viscosity = 102.7 = 500 Pas. (Note: due to the log scale, small changes in the estimate will result in large changes in viscosity. 13.12 Consider an extruder in which the barrel diameter = 4.5 in and length = 11 ft. The extruder screw rotates at 60 rev/min; it has channel depth = 0.35 in and flight angle = 20°. The plastic melt has a Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

69

shear viscosity = 125 x 10-4 lb-sec/in2. Determine: (a) Qmax and pmax, (b) the shape factor Ks for a circular die opening in which Dd = 0.312 in and Ld = 0.75 in, and (c) the values of Q and p at the operating point. Solution: (a) Qmax = 0.5π2(4.5)2(1)(0.35)sin 20 cos 20 = 34.975(0.342)(0.9397) = 11.24 in3/sec pmax = 6π(4.5)(1)(132)(0.0125)(cot 20)/(0.35)2 = 3139 lb/in2 (b) Given: Dd = 0.312 in., Ld = 0.75 in. Ks = π(0.312)4/128(0.0125)(0.75) = 0.024808 (c) From (a), Qx = Qmax - (Qmax/pmax)p = 11.24 - 0.003581p From (b), Qx = 0.024808p Combining, .024808p = 11.24 - .003581p 0.02839p = 11.24 p = 395.9 lb/in2 Qx = 11.24 - 0.003581(395.9) = 9.82 in3/sec 13.13 An extruder has a barrel diameter = 5.0 in and length = 12 ft. The extruder screw rotates at 50 rev/min; it has channel depth = 0.30 in and flight angle = 17.7°. The plastic melt has a shear viscosity = 100 x 10-4 lb- sec/in2. Find: (a) the extruder characteristic, (b) the values of Q and p at the operating point, given that the die characteristic is Qx = 0.00150 p. Solution: (a) Qmax = 0.5π2(5)2(50/60)(0.3)sin 17.7 cos 17.7 = 30.84(0.3040)(0.9527) = 8.93 in3/sec pmax = 6π(5)(50/60)(144)(0.01)(cot 17.7)/(0.3)2 = 3937.6 lb/in2 Qx = Qmax - (Qmax/pmax)p = 8.93 - 0.002268p (b) Given: die characteristic Qx = 0.0015p Qx = 8.93 - 0.002268p = 0.0015p 0.00377p = 8.93 p = 2370 lb/in2 Qx = 8.93 - 0.002268(2370) = 3.55 in3/sec 13.14 An extruder has a barrel diameter of 3.5 in and a length of 5.0 ft. It has a screw channel depth of 0.16 in and a flight angle of 22°. The extruder screw rotates at 75 rev/min. The polymer melt has a shear viscosity = 65 x 10-4 lb- sec/in2 at the operating temperature of 525°F. The specific gravity of the polymer is 1.2 and its tensile strength is 8,000 lb/in2. A T-shaped cross-section is extruded at a rate of 0.11 lb/sec. The density of water is 62.5 lb/ft3. (a) Find the equation for the extruder characteristic. (b) Find the operating point (Q and p), and (c) the die characteristic that is indicated by the operating point. Solution: (a) Qmax = 0.5π2 D2 Ndc sinA cosA = 0.5π2(3.5)2(75/60)(0.16)sin 22 cos 22 = 4.199 in3/sec pmax = 6πDNLη cot A/dc2 =6π(3.5)(75/60)(60)(0.0065)(cot 22)/(0.16)2 = 989.8 lb/in2 Qx = Qmax - (Qmax/pmax)p = 4.199 - 0.004242p (b) Given: T-shaped cross section extruded at 0.14 lb/sec. Density of polymer ρ = specific gravity of polymer x ρwater =1.2(62.4 lb/ft3) = 75 lb/ft3 Convert to lb/in3: ρ= 75 lb/ft3 /(123 in3/ft3) = 0.0433 lb/in3 Qx = 0.11/0.0433 = 2.540 in3/sec. 2.540 = 4.199 - 0.004242p 0.004242p = 4.199 – 2.540 = 1.659 p = 391.1 lb/in2 (c) Qx = Ks p Ks = Qx/p = 2.540/391.1 = 0.00649 Qx = 0.00649 p

Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

70

Injection Molding 13.12 Compute the percentage volumetric contraction of a polyethylene molded part, based on the value of shrinkage given in Table 13.1. Solution: S = 0.025 for polyethylene from Table 13.1. Volumetric contraction = 1.0 - (1 - .025)3 = 1.0 - 0.92686 = 0.07314 = 7.314% Note that we are not using the parameter S from Table 13.1 in the way it was intended to be used. Its intended use is to compute the oversized dimension of a mold cavity in injection molding. Instead, we are using the shrinkage term to calculate the amount of (volumetric) reduction in size of the part after the polymer is injected into the cavity. In fact, a slightly different shrinkage parameter value may apply in this case. 13.13 The specified dimension = 225.00 mm for a certain injection molded part made of ABS. Compute the corresponding dimension to which the mold cavity should be machined, using the value of shrinkage given in Table 13.1. Solution: S = 0.006 for ABS from Table 13.1. Dc = 225.00 + 225.00(0.006) + 225.00(0.006)2 = 225.00 + 1.35 + 0.0081 = 226.36 mm. 13.14 The part dimension for a certain injection molded part made of polycarbonate is specified as 3.75 in. Compute the corresponding dimension to which the mold cavity should be machined, using the value of shrinkage given in Table 13.1. Solution: S = 0.007 for polycarbonate from Table 13.1. Dc = 3.75 + 3.75(0.007) + 3.75 (0.007)2 = 3.75 + 0.0263 + 0.0002 = 3.7765 in. 13.15 The foreman in the injection molding department says that a polyethylene part produced in one of the operations has greater shrinkage than the calculations indicate it should have. The important dimension of the part is specified as 112.5 ±0.25 mm. However, the actual molded part measures 112.02 mm. (a) As a first step, the corresponding mold cavity dimension should be checked. Compute the correct value of the mold dimension, given that the shrinkage value for polyethylene is 0.025 (from Table 13.1). (b) What adjustments in process parameters could be made to reduce the amount of shrinkage. Solution: (a) Given: S = 0.025, Dc = 112.5 + 112.5(.025) + 112.5(.025)2 = 115.383 mm (b) Adjustments to reduce shrinkage include: (1) increase injection pressure, (2) increase compaction time, and (3) increase molding temperatures. 13.16 An injection molded, polyethylene part has a dimension of 2.500 in. A new material, polycarbonate, is used in the same mold. What is the expected corresponding dimension of the polycarbonate molding? Solution: For polyethylene the shrinkage is 0.025 in/in (from table 13.1). Die Cavity = Dc = Dp + DpS + DpS2 = 2.500 + 2.500(0.025) + 2.500(0.025)2 = 2.564 in For polycarbonate, the shrinkage is 0.007 in/in Part dimension = Dc/(1 + S + S2) = 2.564/(1 + 0.007 + 0.0072) = 2.546 in Other Molding Operations and Thermoforming 13.16 The extrusion die for a polyethylene parison used in blow molding has a mean diameter of 18.0 mm. The size of the ring opening in the die is 2.0 mm. The mean diameter of the parison is observed to swell to a size of 21.5 mm after exiting the die orifice. If the diameter of the blow molded container is to be 150 mm, determine (a) the corresponding wall thickness of the container and (b) the wall thickness of the parison. Solution: (a) rsd = Dp/Dd = 21.5/18.0 = 1.194 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

71

tm = rsd2 td Dp/Dm = (1.194)2 (2.0)(21.5)/150.0 = 0.409 mm (b) tp = rsd2 td = (1.194)2(2.0) = 2.851 mm 13.17 A blow molding operation produces a 6.25 in diameter bottle from a parison that is extruded in a die whose outside diameter = 1.25 in and inside diameter = 1.00 in. The observed diameter swell ratio = 1.24. What is the maximum air pressure that can be used if the maximum allowable tensile stress for the polymer is 1000 lb/in2. Solution: Mean extrusion die diameter Dd = (1.25 - 1.00)/2 = 1.125 in and wall thickness td = (1.25 - 1.0)/2 = 0.125 in Blow molding wall thickness tm = (1.24)3(.125)(1.125)/6.25 = 0.0429 in Maximum air pressure p = 2(1000)(0.0429)/6.25 = 13.73 lb/in2 13.18 A parison is extruded from a die with outside diameter = 11.5 mm and inside diameter = 7.5 mm. The observed die swell is 1.25. The parison is used to blow mold a beverage container whose outside diameter = 112 mm (a standard size 2-liter soda bottle). (a) What is the corresponding wall thickness of the container? (b) Obtain an empty 2-liter plastic soda bottle and (carefully) cut it across the diameter. Using a micrometer, measure the wall thickness to compare with your answer in (a). Solution: (a) Dd = (11.5 + 7.5)/2 = 9.5 mm, and td = (11.5 - 7.5)/2 = 2.0 mm tm = (1.25)3(2.0)(9.5)/112 = 0.331 mm (= 0.013 in) (b) Measured value should be close to calculated value. Some wall thicknesses are less. 13.19 A blow molding operation is used to produce a bottle with a diameter of 2.250 in and a wall thickness of 0.045 in. The parison has a thickness of 0.290 in. The pressure used to inflate the parison is 38.0 lb/in2. The observed die swell ratio is 1.30. (a) What is the required diameter of the parison? (b) What is the diameter of the die? (c) What is the tensile stress in the bottle as it is reaches its inflated size? Solution: (a) Dp = tmDm/tp = (0.045)(2.250)/0.290 = 0.349 in (b) Dd = Dp/rsd = 0.349/1.30 = 0.268 in (c) σ = pDm/(2tm) = 38.0(2.250)/(2(0.045)) = 950 lb/in2 13.20 An extrusion operation is used to produce a parison whose mean diameter = 27 mm. The inside and outside diameters of the die that produced the parison are 18 mm and 22 mm, respectively. If the minimum wall thickness of the blow molded container is to be 0.40 mm, what is the maximum possible diameter of the blow mold? Solution: Dd = (22 + 18)/2 = 20 mm, and td = (22 - 18)/2 = 2 mm rsd = 27/20 = 1.35 Rearranging Eq. (13.25) in text, Dm = rsd3tdDd/tm = (1.35)3(2)(20)/(0.40) = 246 mm 13.21 A rotational molding operation is to be used to mold a hollow playing ball out of polypropylene. The ball will be 1.25 ft in diameter and its wall thickness should be 3/32 in. What weight of PE powder should be loaded into the mold in order to meet these specifications? The specific gravity of the PE grade is 0.90 and the density of water is 62.4 lb/ft3. Solution: Density ρ = specific gravity of polymer x ρwater = 0.90(62.4 lb/ft3) = 56.2 lb/ft3 Convert to lb/in3: ρ= 56.2 lb/ft3 /(1728 in3/ft3) = 0.0325 lb/in3 Volume = π(Do3 - Di3)/6 = 0.16667π[(1.25x12)3 - (1.25x12 - 3/16)3] = 10.91 in3 Weight W = (10.91)(0.0325) = 0.355 lb. 13.22 The problem in a certain thermoforming operation is that there is too much thinning in the walls of the large cup- shaped part. The operation is conventional pressure thermoforming using a positive mold, and the plastic is an ABS sheet with an initial thickness of 3.2 mm. (a) Why is thinning Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

72